A thiazolo[5,4-d ]thiazole-bridged porphyrin organic framework as a promising nonlinear optical material †

Porphyrin-based porous organic frameworks are an important group of materials gaining interest due to their structural diversity and distinct opto-electronic properties. However, these materials are seldom explored for nonlinear optical (NLO) applications. In this work, we investigate a thiazolo[5,4-d ]thiazole-bridged porous, porphyrin framework (Por-TzTz-POF) with promising NLO properties. The planar TzTz moiety coupled with integrated porphyrin units enables eﬃcient p -conjugation and charge distribution in the Por-TzTz-POF resulting in a high nonlinear absorption coeﬃcient ( b = 1100 cm GW (cid:2) 1 ) with figure of merit (FoM) r 1 / r 0 = 5571, in contrast to analogous molecules and material counterparts e.g. metal–organic frameworks (MOFs; b = B 0.3–0.5 cm GW (cid:2) 1 ), molecular porphyrins ( b = B 100– 400 cm GW (cid:2) 1 ), graphene ( b = 900 cm GW (cid:2) 1 ), and covalent organic frameworks (Por-COF-HH ; b = 1040 cm GW (cid:2) 1 and FoM = 3534).

In the realm of nonlinear optics (NLO), molecular porphyrins have unique prominence due to their outstanding optoelectronic properties, large and fast NLO responses, possibility of engineering with metals, and excellent thermo-chemical stabilities, making them suitable for applications in telecommunication, data storage, sensors, and display technologies. 1However, there are still enough opportunities to fine-tune the optical nonlinearities of singular molecular porphyrins, which can be achieved by de novo design of integrated porphyrin units with extended p-conjugations and periodic incorporation of opto-electronically active heterocyclic units. 2 The large p-electron delocalization in heterocycles would offer efficient light absorbability and thus red shifting of their absorption bands along with in-plane facile charge transport, which is crucial for optoelectronic applications like NLO. 3,4 There are few reports on linear conjugated porphyrin oligomers, which have shown excellent NLO response.However, arduous multistep synthesis appears to be the bottleneck toward their development. 5onjugated, porous organic frameworks comprising of porphyrin units (POFs) 6 are of high interest due to their scalable protocols, in addition to excellent chemical stability, diverse functionality, and unique opto-electronic properties.Despite this, few have reported successful introduction of heterocyclic units into porous networks. 7Introduction of fused (bi)heterocyclic units e.g.thiazolo [5,4-d]thiazole (TzTz) into a porous polymeric network is interesting because of their semiconductor characteristics associated with the electron deficient nature, high oxidative stability, and a rigid planar structure. 8Notably, TzTz moieties feature an excellent photoabsorbing ability 9 and strong electron acceptor characteristics; when linked with porphyrin units, they are expected to be highly useful in photo(electro)catalysis and opto-electronics applications. 10Until recently, none of the POFs or COFs composed of porphyrin units have been explored as NLO materials.We recently reported three regioregular crystalline Por-COFs 11 with outstanding NLO activity, which inspired us to further investigate and understand analogous porous materials for advanced NLO applications.
The Por-TzTz-POF was synthesised using the standard solvothermal protocol as described in Section S2, ESI.† To carve out the structure-activity relationship in the porphyrin frameworks, and for comparison, we have synthesized a reported crystalline, Schiff-base analogous Por-CQN-COF by condensation of TFPP and 5,10,15,20-tetrakis(4-aminophenyl)-21H,23Hporphyrin (TAPP) (Fig. 1a).The synthesized porphyrin frameworks were examined via powder X-ray diffraction (PXRD) to investigate their crystallinity and phase purity.From PXRD, it is confirmed that the Por-TzTz-POF is amorphous in nature with a broad reflection at 181 2y (Fig. 1b).However, the Por-CQN-COF is crystalline with the most intense first peak at a low 2y angle of B4.71 corresponding to the (100) reflection, along with other minor peaks (Fig. 1c).To gain further insight into the functional groups and the local bonding modes in the Por-TzTz-POF, we recorded the Fourier Transform Infrared (FT-IR) spectrum, from which, the newly formed heterocyclic CQC bond (1736 cm À1 ) and CQN bond (1594 cm À1 ) can be identified.The near disappearance of CQO stretching vibration of the carbonyl group (expected range 1693 cm À1 ) confirms the condensation of the formyl group of TFPP and DTO to form the (bi)heterocyclic TzTz linkages.Furthermore, the FT-IR spectrum shows minor bands corresponding to the -CQN and -C-S bonds of the TzTz ring (Fig. S3, ESI †).The framework structure and composition of the Por-TzTz-POF were confirmed by 13 C cross-polarization magic-angle spinning (CP-MAS) NMR spectroscopy (Fig. 2a).All distinct signals can be assigned to the respective carbon atoms of the porphyrin framework.The spectrum of the Por-TzTz-POF shows the presence of aromatic groups (a chemical shift region of ca.110-150 ppm) as well as higher chemical shifts for the carbons of the (bi)heterocyclic TzTz ring, d = B170 ppm (S-CQN) and 152 ppm (CQC).
The thermal stability of the Por-TzTz-POF was verified using thermogravimetric analysis (TGA) under an N 2 atmosphere.Mass loss shows that about 7% of residual solvent molecules were trapped inside the Por-TzTz-POF, which were removed upon gradual heating to B150 1C.Overall, the framework was stable up to B470 1C.After decomposition, a weight loss of B50% for the Por-TzTz-POF was observed until the end of the scan (Fig. S4, ESI †).N 2 adsorption/desorption analysis of the Por-TzTz-POF displays a typical reversible type-II isotherm with a rapid uptake at low relative pressures giving rise to a BET surface area of 740 m 2 g À1 (Fig. 2b).This value is comparatively higher than those of most of the TzTz-linked POFs reported in the literature such as 604 m 2 g À1 (TzTz-POP-3), 491 m 2 g À1 (TzTz-POP-5), 299 m 2 g À1 (TzTz-POP-1) and 488 m 2 g À1 (TzTz-POP-2). 12The pore size distribution (PSD) was derived from the N 2 adsorption data for the Por-TzTz-POF using nonlocal density functional theory (NLDFT), which suggests narrow micropores of these polymeric frameworks with a major pore diameter of 1.3 nm.This is slightly smaller than the pore diameter value obtained (1.6 nm) from the ideal structure model (Fig. S5, ESI †).The external morphology of the Por-TzTz-POF was visualized by scanning electron microscopy (SEM), which revealed small particles (B30-50 nm), with cubic morphology, for large agglomerations (Fig. S6a and b, ESI †).A similar morphology was also observed in transmission electron microscopy (TEM) images (Fig. 2d and Fig. S6c and d mentioning that the particle size and shape of any organic porous materials synthesized via the solvothermal method are hard to predict and drastically vary due to a range of interactions such as p-p stacking, van der Waals interactions etc.

, ESI †). It is worth
The optoelectronic properties such as UV-vis absorption and photoluminescence (PL) measurements of the Por-TzTz-POF were accessed using the center mount position of an integrating sphere in the dispersion state (2-propanol).The UV-vis spectral studies display all four Q-band components [500-700 nm: Q y (1,0), Q y (0,0), Q x (1,0), Q x (0,0)] for the Por-TzTz-POF (Fig. 2c).The Soret B-band (B(0,0)) is associated with a single component of 418 nm (dominant major peak) similar to the reported Por-CQN-COF. 11However, an additional shoulder peak appears at 442 nm for the Por-TzTz-POF in contrast to the Por-CQN-COF, which corresponds to the TzTz group.We observed an emission at 655 nm in the PL analysis (Fig. 2c), which is identical to that of the reported Por-CQN-COF compound.The fluorescence decays can be fitted with (bi)exponential functions (Fig. 2e) and the amplitude weighted average lifetime for the Por-TzTz-POF is 7.5 ns [t 1 = 0.41 ns (12.2%) and t 2 = 8.46 ns (87.8%)], which is lower than that of the Por-CQN-COF (t avg = 9.17 ns).
In light of the exciting opto-electronic features of the Por-TzTz-POF, the NLO response was examined by the open aperture Z-scan technique at an excitation wavelength of 532 nm from a frequency doubled Nd:YAG laser with varying input intensities.A purely intensity dependent, nonlinear absorption mechanism was observed from the Z-scan profiles at different input intensities (Fig. 3a).For comparison, the NLO response of Por-CQN-COF 11 is also presented in Fig. 3b.Interestingly, it has been found that both the porphyrin frameworks exhibit NLO switching behavior as the nonlinear absorption swap from saturable absorption (SA) to reverse saturable absorption (RSA) with increasing input intensity.Fig. 3 denotes the open aperture Z-scan curves for the (a) Por-TzTz-POF and (b) Por-CQN-COF at peak intensities of 0.04, 0.06 and 0.25 GW cm À2 .At a lower intensity of 0.04 GW cm À2 , both materials showed SA behavior.As the input intensity increases, the excited state absorption leads to characteristic RSA behaviour as depicted in Fig. 3.However, in the case of the Por-CQN-COF, at an input intensity of 0.25 GW cm À2 , an optical switching behavior switch from RSA to SA is observed and is attributed to the dominant excited state absorption at lower intensities (far-focus) and saturation of excited states at higher intensity (near-focus).To further support this hypothesis, the known theoretical model was applied with five level rate equations (Section S5, ESI †). 14 It has been found  that the experimental results are in good agreement with the theoretical fits at different input intensities (Fig. 3).From the fitting results, the nonlinear absorption coefficient (b), ground state absorption cross section (s 0 ), first excited state (s 1 ) and second excited state absorption cross sections (s 2 ) have been determined for both Por-TzTz-POF and Por-CQN-COF.A slightly higher b value is observed for the Por-TzTz-POF (b = 1100 cm GW À1 ) compared to the Por-CQN-COF (b = 1040 cm GW À1 ) (Table S1, ESI †), and the value is much higher than those of many other reported materials such as metalated porphyrins (b = 132-366 cm GW À1 ), MOFs (b = 0.28-0.46cm GW À1 ) and graphene (b = 900 cm GW À1 ). 11,14,15We assume that the higher NLO response of the Por-TzTz-POF could be attributed to a combined effect of the structural planarity of the TzTz-phenyl core (quasi-planar: dihedral angle 6.91), effective inter-layer stacking, efficient p-conjugation-electron transport and framework disorderliness (loss of symmetry) compared to the imine (CQN)-phenyl core (dihedral angle 62.81) in the case of the Por-CQN-COF (Fig. S9, ESI †). 12 Moreover, the obtained figure of merit (FoM = s 1 /s 0 ; 5571) for the Por-TzTz-POF is also higher than that of our recently reported porphyrin based COFs; Por-COF-HH (FoM = 3534), Por-COF-ZnCu (FoM = 3565) and Por-COF-ZnNi (FoM = 3762), tabulated in Table S2 (ESI †). 11Overall, these results signify a structure-activity relationship in porphyrin based porous organic materials that can be useful in optical switching applications. 16,17n summary, we have synthesized a conjugated TzTz-linked porphyrin organic framework employing single-step direct condensation of A4 porphyrin tetra-aldehyde and DTO.Moreover, to prove the concept and to draw the benefits from infinite conjugated porphyrin networks, the NLO response of the Por-TzTz-POF has been investigated using the Z-scan technique.Next, the NLO activity of the Por-TzTz-POF was compared with that of a reported analogous crystalline Schiff base Por-COF (Por-CQN-COF).Although, optical switching behavior from SA to RSA with input intensity was observed for both materials, the amorphous Por-TzTz-POF is found to display higher nonlinear absorption coefficient values (b = B1100 cm GW À1 and FoM = 5571).Through this work, we tried to establish a structureactivity relationship in porphyrin containing organic frame-

Fig. 1
Fig. 1 Schematic representations of the synthesis of the Por-TzTz-POF and Por-CQN-COF (previously reported as Por-COF-HH), 11 (b) and (c) experimental (red) PXRD profiles of the Por-TzTz-POF and Por-CQN-COF (the black pattern is the simulated one derived from the eclipsed model) respectively with molecular models (C: grey; N: blue; S: yellow and H: white).

Fig. 3
Fig. 3 Open aperture Z-scan traces for (a) Por-TzTz-POF and (b) Por-CQN-COF 11 under the excitation at 532 nm, ns laser at different input intensities.The solid lines represent the theoretical fitting, and triangles, spheres and hexagons represent the experimental data.

Fig. 2
Fig. 2 (a) 13 C cross-polarization magic-angle spinning (CP-MAS) solid state NMR spectra of the Por-TzTz-POF; (b) N 2 physisorption isotherms collected at 77 K; (c) UV-vis and photoluminescence spectrum (measured in the integration sphere in the dispersion state in 2-propanol); (d) TEM images of the Por-TzTz-POF (scale bar = 50 nm); and (e) time-correlated single-photon counting experiment for the Por-TzTz-POF measured in 2-propanol.The sample was excited with a l ex = 380 nm laser and emission was measured at l em = 655 nm.